Telechargé par Cali Chen

# induction heating theory

publicité
```INDUCTION HEATING was first noted when it was found that heat
was produced in transformer and motor windings, as mentioned in the
Chapter “Heat Treating of Metal” in this book. Accordingly, the theory of
induction heating was studied so that motors and transformers could be
built for maximum efficiency by minimizing heating losses. The development of high-frequency induction power supplies provided a means of
using induction heating for surface hardening. The early use of induction
involved trial and error with built-up personal knowledge of specific
applications, but a lack of understanding of the basic principles. Throughout the years the understanding of the basic principles has been expanded,
extending currently into computer modeling of heating applications and
processes. Knowledge of these basic theories of induction heating helps to
understand the application of induction heating as applied to induction
heat treating. Induction heating occurs due to electromagnetic force fields
producing an electrical current in a part. The parts heat due to the resistance to the flow of this electric current.
Resistance
All metals conduct electricity, while offering resistance to the flow of this
electricity. The resistance to this flow of current causes losses in power that
show up in the form of heat. This is because, according to the law of conservation of energy, energy is transformed from one form to another—not lost.
The losses produced by resistance are based upon the basic electrical formula: P = i2R, where i is the amount of current, and R is the resistance.
Because the amount of loss is proportional to the square of the current, doubling the current significantly increases the losses (or heat) produced. Some
metals, such as silver and copper, have very low resistance and, consequent-
6 / Practical Induction Heat Treating
ly, are very good conductors. Silver is expensive and is not ordinarily used
for electrical wire (although there were some induction heaters built in
World War II that had silver wiring because of the copper shortage). Copper
wires are used to carry electricity through power lines because of the low
heat losses during transmission. Other metals, such as steel, have high resistance to an electric current, so that when an electric current is passed through
steel, substantial heat is produced. The steel heating coil on top of an electric
stove is an example of heating due to the resistance to the flow of the household, 60 Hz electric current. In a similar manner, the heat produced in a part
in an induction coil is due to the electrical current circulating in the part.
Alternating Current and Electromagnetism
Induction heaters are used to provide alternating electric current to an electric coil (the induction coil). The induction coil becomes the electrical (heat)
source that induces an electrical current into the metal part to be heated
(called the workpiece). No contact is required between the workpiece and
the induction coil as the heat source, and the heat is restricted to localized
areas or surface zones immediately adjacent to the coil. This is because the
alternating current (ac) in an induction coil has an invisible force field (elec-
Fig. 2.1 Induction coil with electromagnetic field. OD, outside diameter; ID,
inside diameter. Source: Ref 1
https://dw-inductionheater.com
[email protected]
Theory of Heating by Induction / 7
tromagnetic, or flux) around it. When the induction coil is placed next to or
around a workpiece, the lines of force concentrate in the air gap between the
coil and the workpiece. The induction coil actually functions as a transformer primary, with the workpiece to be heated becoming the transformer
secondary. The force field surrounding the induction coil induces an equal
and opposing electric current in the workpiece, with the workpiece then heating due to the resistance to the flow of this induced electric current. The rate
of heating of the workpiece is dependent on the frequency of the induced
current, the intensity of the induced current, the specific heat of the material,
the magnetic permeability of the material, and the resistance of the material
to the flow of current. Figure 2.1 shows an induction coil with the magnetic
fields and induced currents produced by several coils. The induced currents
are sometimes referred to as eddy-currents, with the highest intensity current
being produced within the area of the intense magnetic fields.
Induction heat treating involves heating a workpiece from room temperature to a higher temperature, such as is required for induction tempering or
induction austenitizing. The rates and efficiencies of heating depend upon
the physical properties of the workpieces as they are being heated. These
properties are temperature dependent, and the specific heat, magnetic permeability, and resistivity of metals change with temperature. Figure 2.2
shows the change in specific heat (ability to absorb heat) with temperature
Fig. 2.2 Change in specific heat with temperature for materials. Source: Ref 2
8 / Practical Induction Heat Treating
for various materials. Steel has the ability to absorb more heat as temperature increases. This means that more energy is required to heat steel when it
is hot than when it is cold. Table 2.1 shows the difference in resistivity at
room temperature between copper and steel with steel showing about ten
times higher resistance than copper. At 760 &deg;C (1400 &deg;F) steel exhibits an
increase in resistivity of about ten times larger than when at room temperature. Finally, the magnetic permeability of steel is high at room temperature,
but at the Curie temperature, just above 760 &deg;C (1400 &deg;F), steels become
nonmagnetic with the effect that the permeability becomes the same as air.
Hysteresis
Hysteresis losses occur only in magnetic materials such as steel, nickel,
and a few other metals. As magnetic parts are being heated, such as those
made from carbon steels, by induction from room temperature, the alternating magnetic flux field causes the magnetic dipoles of the material to
oscillate as the magnetic poles change their polar orientation every cycle.
This oscillation is called hysteresis, and a minor amount of heat is produced due to the friction produced when the dipoles oscillate. When steels
are heated above Curie temperature they become nonmagnetic, and hysteresis ceases. Because the steel is nonmagnetic, no reversal of dipoles can
Table 2.1
Resistivity of different metals
Approximate electrical resistivity, &micro;K &middot;cm (&micro;K &middot;in.), at temperature, &deg;C (&deg;F), of:
20 (68)
Material
Aluminum
Antimony
Beryllium
Brass(70Cu-30Zn)
Carbon
Chromium
Copper
Gold
Iron
Magnesium
Manganese
Mercury
Molybdenum
Monel
Nichrome
Nickel
Platinum
Silver
Stainless steel,
nonmagnetic
Stainless steel 410
Steel, low carbon
Steel, 1.0% C
Tin
Titanium
Tungsten
Uranium
Zirconium
95 (200)
2.8
(1.12)
...
39.4
(15.5)
...
6.1
(2.47)
...
6.3
(2.4)
...
3353
(1320.0)
...
12.7
(5.0)
...
1.7
(0.68)
...
2.4
(0.95)
...
10.2
(4.0)
14.0 (5.5)
20.8
(8.2)
27.4 (10.8)
4.5
(1.76)
...
185
(73.0)
...
9.7
(3.8)
...
5.3
(2.1)
...
44.2
(17.4)
...
108.0
(42.5)
...
6.9
(2.7)
...
9.9
(3.9)
...
1.59
(0.626)
...
73.7
(29.0)
...
62.2
12.7
18.8
11.4
53.3
5.6
32.0
40.6
(24.5)
(5.0)
(7.4)
(4.5)
(21.0)
(2.2)
(12.6)
(16.0)
...
16.5 (6.5)
22.9 (9.0)
...
...
...
...
...
205 (400)
315 (600)
...
...
...
...
...
...
...
...
...
...
...
...
...
...
...
...
...
...
...
...
6.9 (2.7)
...
...
...
...
...
3.8 (1.5)
...
...
49.8 (19.6)
...
...
...
...
...
114.3 (45.0)
29.2 (11.5)
...
...
99.1 (39.0)
10.4 (4.1)
...
11.4 (4.5)
...
1828.8 (720.0)
...
5.5 (2.15)
...
63.5 (25.0)
...
...
...
...
...
...
...
40.4 (15.9)
...
...
...
540 (1000)
...
...
...
20.3 (8.0)
...
...
...
...
...
...
...
...
...
...
...
...
101.6 (40.0)
59.7 (23.5)
69.9 (27.5)
...
...
...
...
...
760 (1400)
980 (1800)
...
...
...
...
...
...
...
...
...
...
...
...
...
9.4 (3.7)
...
12.2 (4.8)
106.7 (42.0) 123.2 (48.5)
...
...
...
...
...
...
...
...
...
...
...
...
114.3 (45.0)
...
...
54.4 (21.4)
...
...
6.7 (2.65)
...
...
130.8 (51.5)
102
108
...
(40.0)
(42.5)
...
...
...
...
...
127 (50.0)
115.6 (45.5)
121.9 (48.0)
...
...
...
...
...
1205 (2200)
...
...
...
...
...
...
...
...
...
...
...
...
...
33.0 (13.0)
...
...
...
...
...
...
...
121.9 (48.0)
127.0 (50.0)
...
165.1 (65.0)
38.6 (15.2)
...
...
Source: Ref 3
https://dw-inductionheater.com
[email protected]
Theory of Heating by Induction / 9
Fig. 2.3 Effect of hysteresis on heating rate. N, north; S, south; B, flux density
in a ferromagnetic material; H, corresponding magnetic intensity.
Source: Ref 4
occur. Figure 2.3 shows an illustration of hysteresis and the effect on the
magnetic flux field strength. Figure 2.4, as represented by the line
“ABCD,” shows the Curie temperature for carbon steels.
Skin Effect and Reference Depth
Induction heating occurs when an electrical current (eddy current) is
induced into a workpiece that is a poor conductor of electricity. For the
induction heating process to be efficient and practical, certain relationships of the frequency of the electromagnetic field that produces the eddy
currents, and the properties of the workpiece, must be satisfied. The basic
nature of induction heating is that the eddy currents are produced on the
outside of the workpiece in what is often referred to as “skin effect” heating. Because almost all of the heat is produced at the surface, the eddy currents flowing in a cylindrical workpiece will be most intense at the outer
surface, while the currents at the center are negligible. The depth of heating depends on the frequency of the ac field, the electrical resistivity, and
the relative magnetic permeability of the workpiece. For practical purposes of understanding, the skin heating effect (reference depth) is defined as
the depth at which approximately 86% of the heating due to resistance of
the current flow occurs. Figure 2.5 shows reference depths for various
materials at different temperatures. The reference depths decrease with
higher frequency and increase with higher temperature. The reference
depth, as mentioned, becomes the theoretical minimum depth of heating
that a given frequency will produce at a given power and workpiece temperature. The cross-sectional size of the workpiece being heated must be
at four times the reference depth, or what appears to be current cancella-
10 / Practical Induction Heat Treating
Fig. 2.4 Curie temperature for carbon steels. Source: Ref 2
Fig. 2.5 Reference depth for various materials. Source: Ref 2
https://dw-inductionheater.com
[email protected]
Theory of Heating by Induction / 11
tion occurs. Figure 2.6 shows the critical frequency (or minimum frequency) for heating different bar diameters. Figure 2.7.a illustrates three examples of ratios of workpiece thickness (a) and reference depth of heating (d)
with the respective current distribution. The dashed lines show exponential
decay from either side, while the solid line gives the net current from the
summation of the two dashed lines. As the workpiece thickness/reference
depth of heating ratio decreases below four to one, the net current decreases. The net heating curves (Fig. 2.7.b) are obtained by squaring the net
current density, demonstrating that when a/d = 4, the best surface heat
distribution occurs.
For a fixed frequency, the reference depth varies with temperature
because the resistivity of conductors varies with temperature. With magnetic steels the magnetic permeability varies with temperature, decreasing
to a value of one (the same as free space) at the Curie temperature, at
which steel becomes nonmagnetic. Because the reference depth increases
when steel is heated over the Curie temperature, the a/d ratio of 4 when
austenitizing must be based on the reference depth when the steel is at a
temperature above the Curie. Figure 2.8 shows an illustration of the deeper depth of current penetration over the Curie. Because of these effects the
reference depth of nonmagnetic materials may vary by a factor of two or
three over a wide heating range, whereas for magnetic steels it can vary by
a factor of 20. The net effect is that cold steel has a very shallow reference
depth as compared to hot steel.
Fig. 2.6 Critical frequency for efficient heating of several materials. Source:
Ref 2
12 / Practical Induction Heat Treating
(a)
(b)
Fig. 2.7 (a) Ratios of object thickness, a, and reference depth, d. (b) Net
Penetration depth, 
heating curves. Source: Ref 5
Curie point
Temperature
Fig. 2.8 Variation of current penetration depth through Curie. Source: Ref 6
https://dw-inductionheater.com
[email protected]
Theory of Heating by Induction / 13
Another very important result of the skin effect is evidenced in heating
efficiency. Heating efficiency is the percentage of the energy put through
the coil that is transferred to the workpiece by induction. As shown in
Fig. 2.7, if the ratio of workpiece diameter to reference depth for a round
bar drops below about 4 to 1, the heating efficiency drops. This ratio
becomes what is defined for round bars as the critical frequency for
heating. Figure 2.9 shows the critical frequency as a function of diameter for round bars and Figure 2.10 shows the efficiency of heating as a
function of this critical frequency. Higher frequencies are needed to efficiently heat small bars, but as Figure 2.10 shows, once the critical frequency is reached, increasing the frequency has very little effect on relative efficiency.
For through heating, a frequency close to the critical frequency should
be selected so that the workpiece will through heat faster. In contrast for
case hardening, frequencies higher than the four-to-one ratio will be
selected based on a combination of being both higher than the critical frequency and high enough to generate the desired skin effect heating for
Fig. 2.9 Critical temperature as a function of diameter for round bars. Source:
Ref 2
14 / Practical Induction Heat Treating
Fig. 2.10 Efficiency of heating as a function of frequency. Source: Ref 2
production of the specified case. Once the critical frequency is reached,
the case depth requirements will help in frequency selection because
lower frequencies have deeper reference depths, thereby producing deeper
case depths. The Chapter “Induction Heat Treating Process Analysis” in
this book discusses frequency selection.
Power Density
Selection of power is just as important as the selection of frequency.
When case hardening is to be done, the short heat cycles that are necessary
require higher power density (energy input per unit of surface) than
through-heating applications. The power density at the induction coil is
the metered output power divided by the amount of workpiece surface
within the induction coil and is expressed in kW/cm2 or kW/in.2. Power
density requirements, as shown subsequently, can be used to rate the
power requirements for an application.
Power requirements are related to the amount of energy required to heat
a workpiece and to the induction heating system power losses. The energy
or heat content required to heat the workpiece can be calculated when the
https://dw-inductionheater.com
[email protected]
Theory of Heating by Induction / 15
material, its specific heat, and the effective weight of material to be heated
per hour are known.
The value kWh is (lbs/hour &times; specific heat &times; temperature rise)/ 3413,
where the pounds per hour relate to (3,600 seconds &times; part weight)/actual
heat cycle. Heat input required to heat a specific workpiece represents
only the energy or power that needs to be induced from the coil into the
workpiece. Other system losses such as coil losses, transmission losses,
conversion losses, and the ability to load match for required output power
determine the power supply rating. Table 2.2 shows the typical system
losses for a typical solid-state power supply system and a radio frequency
(RF) vacuum tube system. Through calculation of the heat content
requirements of the workpiece at the coil, and with the system losses
known, the power requirements for heating can be determined. If a heat
content of 25 kWh is needed by the workpiece and system losses are 50%,
then a minimum output power rating of 50 kW is needed from the power
supply. As discussed in the Chapter, “Induction Heat Treating Systems” in
this book, the ability of a power supply to produce rated output power
depends on the ability to load match the power supply to the induction
coil. When in doubt it is advisable, to use power supplies with higher output power ratings than needed. The Chapter “Induction Heat Treating
Process Analysis” in this book deals with the determination of power supply ratings from tables that have been developed through calculation and
correlation with surface power densities and for through heating. From
calculation of the surface of the area to be heated in relationship to power,
power density curves define power supply ratings. For instance if a power
density of 1.55 kW/cm2 (10 kW/in.2) is needed and the area to be heated is
5 square inches, then the power required is 50 kW. In general, obtaining
higher production rates for specific case depths for surface hardening
requires higher power densities.
Through heating systems can be defined from knowing the crosssectional size and the weight of steel to be heated per hour. Lower power
densities and frequencies are used for through heating because the workpieces need to have the heat soak and penetrate to the core. Higher productivity is obtained from using more power heating and from heating more
workpiece area at the same time, thereby not increasing the power density.
Higher power densities provide the ability to heat surfaces more rapidly. However, there may be limitations to the amount of power that an
individual induction coil can handle. Induction coil design is discussed in
Table 2.2
Typical system losses for different induction power supplies
Power supply
Frequency
Terminal
efficiency, %
Solid state
10 kHz
450 kHz
90
65
Source: Ref 7
Output
transformer
efficiency, %
Coil
efficiency, %
System
efficiency,%
75
60
75
85
51
33
16 / Practical Induction Heat Treating
the Appendix “Induction Coil Design and Fabrication” in this book. The
amount of cooling water a given coil can carry defines the amount of
power it can carry. Also, the fact that the power supply has a more than
adequate power rating does not necessarily mean that the power can be
induced into the workpiece. Only 125 kW of a 250 kW power supply
may load into a given coil and part. Load matching and tuning are discussed in the Chapter “Induction Heat Treating Systems” in this book.
Tables of power densities are listed in that Chapter as well, and tables of
scanning speeds are listed in the Appendix “Scan Hardening” in this
book.
Conduction of Heat
The primary mechanism of heat flow to the interior of a workpiece
comes from the conduction of the heat first produced by the eddy currents on the surface. Hysteresis produces a secondary effect and is a
small, second producer of heat. Losses due to hysteresis are usually
ignored in the heat content calculations for induction processing because
of the minor effect. As previously discussed, the heating rate is mainly
affected by:
•
•
•
Field strength of the magnetic flux field
Coupling of the induction coil to the workpiece
The electrical and magnetic properties of the material being heated
The desired rate of heating varies with the application. Mathematical
analysis of heat transfer can be quite complex because of the interreaction of the intense heat produced due to the eddy-current heating of
the surface, the rate of heat transfer toward the core, and the fact that the
electrical, thermal, and metallurgical properties of most materials
exhibit a strong dependence on temperature and vary during the heating
cycle.
One way to view the heat propagation is as a wave format. Using carbon
steel as an example, high heat is first produced in the reference depth of
the magnetic material. When the Curie temperature is passed, the depth
being heated increases in a wavelike motion until the reference depth of
the nonmagnetic material is reached. From that point most of the heat
transfer occurs by the inward conduction of heat. Figure 2.11 shows the
temperature profile of heat for 25 kHz on a 50 mm (2 in.) cylinder. At 0.4
s the surface being heated is being heated under the Curie and is nonmagnetic. At 1.15 s the surface is nonmagnetic, and the surface is heating
deeper with minor temperature migration into the core. At 6.5 s the
austenitic portion of the surface has increased to about 0.200 in. deep, and
there has been minor temperature migration to the core. It should be noted
https://dw-inductionheater.com
[email protected]
Theory of Heating by Induction / 17
Fig. 2.11 Interrelationship among heating time, power density, and hardened depth. Source: Ref 6
that at this point in order to accomplish the heat transfer, the surface temperature has increased to 1200 &deg;C (2192 &deg;F). Heat transfer is a matter of
temperature differential and the thermal conduction rate of the workpiece.
When the material is austenitic, higher temperature differential is necessary at the surface to increase the speed of heat conduction and transfer
toward the core. As soon as the power is turned off, the increase in temperature seems to stop at the edge of the austenitized area. When heat
treating parts, the case depth produced during heating does not appear to
penetrate any deeper while the part is being quenched (except in the circumstance of small diameter parts). During case hardening, cooling
occurs from both the outer surface on which the quenchant is being
applied, and the core towards which the heat is migrating. Holes under the
case can affect both the eddy-current distribution and heat transfer. This is
discussed in the Chapter “Induction Heat Treating Process Analysis” in
this book.
The important thing to remember in frequency selection is that smaller
parts need higher frequencies, and that the lowest frequency that will heat
a given cross section is usually the most economical.
18 / Practical Induction Heat Treating
REFERENCES
1. Heat Treating, Vol 4, Metals Handbook, 9th ed., American Society for
Metals, 1981
2. S.L. Semiatin and D.E. Stutz, Induction Heat Treating of Steel, American Society for Metals, 1986
3. S.L. Semiatin and S. Zinn, Induction Heat Treating, ASM International, 1988
4. C.A. Tudbury, Basics of Induction Heating, John F. Rider, Inc., New
Rochelle, NY, 1960
5. Heat Treating, Vol 4, ASM Handbook, ASM International, 1991
6. V. Rudnev et al., SteelHeat Treatment Handbook, Marcel Dekker, Inc.,
1997
7. R.E. Haimbaugh, Induction Heat Treating Corp., personal research
https://dw-inductionheater.com
[email protected]
```